|Top Down Approach|
|Swords are usually polished to a high sheen. Even wootz blades or composition blades, where you want to see a pattern and not a mirror-like surface, need to be polished first so the pattern can be revealed in a second step.|
|Stefan Mäder asserted in his voluminous and
work (I'll get back to it later) that with respect to polishing nothing can
rival the perfection achieved by specialized Japanese craftsmen using
century-old methods for polishing sword blades.
That's baloney, of course. Any standard silicon wafer has been polished to a perfection far exceeding that of a katana.
|Let's start by considering polishing as a
technique that is not only used for sword blades but for all kinds of materials
as part of a production process. Note that
I use the word "polishing" for all methods that flatten a surface
including terms like grinding or lapping. To understand what polishing is all
about, I will go through a number of polished products, always asking three
|1. Example: You polish your pyramid in order to achieve a pleasant looking smooth surface. Moreover, you may polish some of the building blocks because it is easier to do precision building with blocks that have "polished" and parallel sides.|
|So why did
ancient Egyptian guys polish those stones about 4.500 years ago (besides that
their Pharaoh made them)? Because your pyramid just looked that much cooler
1) with polished sides.
How did they assess the quality of the polished surface? They looked. In addition, they moved some straight rod across the surface and looked if there were major deviations.
And we know how it was done: with copper and stone tools and lots of sweat.
|Now you are going to tell me that flattening the sides of humongous pyramid is not really polishing, it's just flattening the sides of a pyramid. So what is polishing for you? I guess I know. So here is example No. 2|
|Example 2. Let's make a mirror. We need mirrors so the wife can make herself pretty for you.|
|In other words: we want to make a device that interacts with visible light in a defined way. Here are some mirrors with various degrees of perfection:|
mirror does two things:
|Mirrors can be flawed for two reasons:
|So why do we
need mirrors? Well, besides the needs of the females of the species there are
many uses for mirrors in science and technology. I'm sure you can come up with
examples of your own.
How do we assess the quality of a mirror? I've covered that already; see above.
|How is it
done? How do we make a mirror? Now there is a good a question. There are
essentially two ways
|What else do we learn from looking at those mirrors? We learn that when you talk about polishing, you must define the scales you are considering. If the surface of a pyramid is flat within 15 mm over 150 m = 150.000 mm, it is just as well polished as your sword that is flat within 3 µm over a distance of 3 cm = 30.000 µm.|
|So far we went "top down" - from large polished structures to smaller ones. Now let's go bottom up!|
|Bottom Up Approach and "Theory" of Polishing|
|As a third example let's look at the ultimate: X-ray mirrors. There are various kinds of X-ray mirrors; the one I have in mind is a sequence of perfectly flat thin layers of two different materials. In cross-section it looks like this:|
|The alternating layers are tungsten (W; dark) and carbon (C; bright), respectively, on a silicon (Si) substrate. Look at the scales to get an idea about layer thickness and interface flatness. In the lower picture you see the "atoms" of the silicon! These mirrors are good mirrors only if they are as flat as possible. How flat is that? Well - remember our basic view of the universe? All that exists around us (including us) consists of atoms and photons. Nothing else. The size of an atom gives the smallest possible scale on which to judge roughness. Taking this into account, it is easy to see where the limits are.|
|You have a perfect single crystal with the surface being a major plane of the crystal lattice. The remaining roughness amplitude then is about half the size of an atom or about 0.1 nm. You can't do better than this and the X-ray mirror from above comes pretty close.|
|However, in real life there is (almost) no such thing as a crystal surface as shown above. In real life the crystal shown above would schematically look like this:|
|The surface is typically oxidized. If that happened in normal (and thus very dirty) air, the oxide might include tiny "dirt" particles that floated around. The oxide surface might be a bit rougher than the original surface but doesn't have to be. You may not notice that "native" oxide on many polished products, and it is typically a good thing to have because it protects the underlying materials.|
|Since we usually do not have single crystals, and since the grains are usually oriented randomly, we encounter situations like that for the ultimate limit of regular crystalline materials:|
|Of course, you would also have to add the oxide-and-dirt layer as above; I was just to lazy to draw that too.|
|Now let's look at scales. When you polish your sword (or pretty much everything else), in order to achieve the effect you are after, you essentially must be aware of three scales (here I go again). The figure below illustrates that.|
|1. The "large" scale. This is a scale far larger than what you go for by polishing. It is determined not by your polishing method but by the general shape of you artifact. In other words: if your sword is bend, no amount of polishing for the mirror sheen will make it straight.|
|2. The intermediate scale or the important scale. In the figure I have shown it kind
of saw-toothed, indicating that it may have been caused by something like
grinding in one direction. Of course, the valleys and protrusions can have
other shapes, too.
This is the scale that determines how good your polishing is in relation to what you want to achieve.
|3. The fine scale. That is the scale that is unimportant
for your needs. You simply won't "see" it.
Of course, if the intermediate scale must already be as small as possible, i.e. on an atomic scale, there is no unimportant smaller scale any more.
|The question now is: What defines the intermediate scale? The answer is simple: It depends on what you use to "look" at the polished surface. Once more going back to the basic law of the universe: All you have to "look" at some surface with are optical photons. I, on the other hand, also have all kinds of other photons (e.g. from X-rays) at my disposal, plus atoms and their constituents (i.e. elementary particles). I can hurl whatever I like onto a polished surface to "see" what it is like. A great way of doing that is to use electrons in a scanning electron microscope, for example.|
|What I'm going to "see" simply depends on the size of my probe. If I throw atoms at a surface, the way they will bounce back responds to roughness on an atomic scale. A probe atom hitting one of the ledges in the figure above will bounce back differently than atoms hitting the flat region. It "sees" roughness on a scale comparable to its own size.|
|So what is the size of light? It's given by its wavelength, of course. That's a quite general truth because everything, including all particles, can be described as a wave.|
|Light that our eyes can detect has wavelengths from 400 nm - 700 nm or roughly somewhat less than 1 µm. What follow is|
|Roughness values of 100 nm or so are "much
smaller" (that's what "<<" means) than 1 µm. In other
words: The "fine scale" roughness of your sword blade could still
amount to 100 nm between the ups and downs, equal to several hundreds of atoms
piled on top of each other - and you wouldn't notice it by "just
In contrast, "looking" with X-rays (wavelengths around nm) demands that your surface must be as flat as possible, i.e. atomically flat, if you want it to be a good mirror. Contrarwise, to radio waves (wavelengths of m) the surface of buildings or the earth in general "looks" highly polished and acts as a good mirror.
|Basic Ways of Polishing|
|It remains to look at how polishing is done. As far as sword blades are concerned, we need to look at the large scale and the intermediate scale.|
|The meaning of the large scale is clear. The
sides of the blade should show no bending, bulges or waviness other than that
intended. If you use it as mirror, it should distort the image only as given by
the intended geometry. Proper "polishing" or better
grinding is then achieved with "grinding
wheels". It certainly takes some skill to grind evenly (and to keep your
grindstone in good order) but it is not too difficult.
Every smith had a grinding wheel that may have looked like this:
|The difficult part is too polish to a "bright sheen", or as we know now, to a roughness well below 1 µm.|
|There are two
completely different ways for doing that.
|The first method is quick and easy, the second method is slow, difficult, and problem ridden - but it is what we need to do in most cases. The polished specimen might look identical for both methods but if you look a bit more closely (with an electron microscope, for example) you see major structural differences. Very schematically, this is what you get with brush polishing|
|When you polish with a "brush", you
simply deform the uneven surface by
applying high local stress. You can do
this even with a "soft" brush because you apply force to the small areas of the protruding ridges and peaks of
the material that stick out from the bulk if you have a rough surface. Metals
yield and the
protruding material is essentially "smeared around" by
deformation. Microcracks will also develop, and a lot of vacancies will be
You do flatten the surface but at the expense of creating a heavily damaged surface layer, typically several micrometers thick, and full of dislocations, microcracks, vacancies and whatever other defects are possible.
Brittle materials are not so easy to "brush polish". If it works, you are also left with a damaged surface region.
Your coarse light beams (the wavelength would be about 100 times larger then the figure above) will not notice that. The surface is shiny and mirror-like. If that is all you care for, brush polishing is fine.
|What we frequently need, however, must look like this:|
|The surface has the same roughness and thus optical appearance as the brush-polished one above, but the crystal lattice is intact and perfect up to the last atom. I omitted the oxide layer; it doesn't change the essentials.|
|Why would we want to go for that, if it doesn't look any different and is so much more difficult to do? There are a number of reasons:|
|1. You want to judge the quality of a blade by looking at it. Then you must be able to see the basic structure and the defects in the blade and not just an irrelevant damaged top layer. That's why Japanese swords had to be slurry polished. Experts then could judge the quality of a blade.|
|2. You want to reveal the internal structure of a blade, for example a wootz pattern or the pattern created by forging a composite sword. This is done by "differential etching", by dissolving different constituents of a blade (harder vs. softer steel, steel vs. cementite, ferrite vs. martensite...) with different rates. This creates a pattern on the surface that you can see. Traditionally, you use natural liquids like fruit juices, or vinegar as etchants. This obviously can't work on damaged surfaces.|
|3. You want to investigate your material (steel or whatever) by defect etching. The same considerations as above apply, just more so because now you look at the specimen with a microscope. You must polish very well, and you use (dangerous) "chemical" etchants" rather than fruit juice.|
|You want to "build" something on top of your polished material. That's one way to describe all of semiconductor technology in one sentence. But is also applies to simple innocent techniques like coating some metal galvanically. Your specimen surface than better is atomically intact as shown above|
|It remains to see how slurry polishing is done.|
|Slurry Polishing and Chemical-Mechanical Polishing|
|A slurry is a mixture of a solid particles and a liquid. A slurry for polishing should contain hard particles with sizes in a well-defined range, for example 1 µm ± 0.3 µm. The particles should be harder than the material you need to polish.|
|The ultimate thus are diamond
slurries. For obvious reasons, they usually cover the small particle size
region. Otherwise you may go for silicon carbide (SiC), aluminum oxide or
(Al2O3), or silicon dioxide (SiO2), also known
or whatever else works for you.
The latter two substances you might find in nature, the others you must make.
|In contrast, a grindstone is a mixture of hard particles embedded in a soft solid matrix. You may find this kind of composite material in nature (typically some kind of sandstone, containing quartz particles in a clay mineral matrix) or you make it.|
|Polishing simply means that a hard particle
removes some of the material to be polished by scratching. The trick is to
scratch more in places where there are protrusions of the material to be
polished. This is done by pressing a flat surface containing the particles on
your specimen. On protrusions you automatically press harder and thus scratch
If you use a grindstone, it is clear how this works. It is also clear that on the large scale, the quality of your polishing depends on the flatness of your grindstone.
|If you use a slurry, you must apply it with some
pressure, and for this you need a polishing
pad. You can use a handkerchief soaked with slurry wrapped over your
finger, or a large round pad of felt, textile, fur or God knows what, that is
glued to a flat round disc that rotates over your specimen.
Using a slurry instead of a grindstone has a couple of advantages:
Here is a commercial machine for polishing silicon wafers (or anxthing else that fits)
|Note that I haven't said that high-quality polishing is easy or cheap! And quite obviously, you can't polish a blade in a machine like that.|
|As long as humankind had to use natural materials for making grindstones and slurries, polishing was an art, especially if you went for optical quality. The famous "Thank You" letter of Theoderic for those cool swords he got from Thrasamond, King of the Vandals, explicitly mentions the quality of the polishing and the "splendid dust granted to your country by the bounty of nature" needed for that.|
|Polishing then consisted of applying grindstones
/ slurries with ever finer grain size of the particles in the slurry. As long
as polishing was done by scratching, the resulting surface roughness was simply
given by the diameter of the particles you scratched with. For a mirror-like
surface you had to go through many stages, the last on with particle sizes well
below 1 µm.
Even today it is not so easy to make particles this small and to keep them suspended in a liquid. Take the wrong liquid and they clump together, for example. If you had a working system of many grades of grindstones / slurries, and you knew how to make them, maintain them and apply them, you kept that a closely guarded secret, of course.
|When our students need to polish a specimen, they
use ready made slurries, polishing pads optimized for the material, and
sophisticated and expensive polishing machines. Nevertheless, they almost
automatically fail to achieve a good polished surface. You simply need to
acquire some experience, a "feel" for what you are doing. If you
never have polished before and just follow detailed instruction, your result
will be like that sweater you knitted for the first time by following
Worse, even if you do everything right, you still end up with a heavily damaged surface layer. Its thickness is roughly equal to the diameter of the particles you used for scratching. As far as polishing swords is concerend, this layer is far thinner then the damaged layer obtained by brush polishing and therfore neither critical for judging sword blades by eye or for "pattern etching".
This damaged layer, however thin, will not allow semiconductor technology, unfortunately. We need to do better.
|One way is to remove the damaged layer by finding an etchant that dissolves the damaged material but not the perfect material. After polishing purely mechanically with 0.1 µm sized particles for example, you only need to remove a damaged layer that's a fraction of a micron thick. That doesn't take long; and you wouldn't be able to see a difference either.|
|You can do even better: Remove the damaged layer in-situ during the polishing procedure. All you need to do is to use some etchant as part of the slurry. A hard particle in the slurry makes a tiny groove by scratching, the region around the groove is heavily damaged, the etchant in the slurry dissolves that region - bingo! You have a perfect surface now.|
|I don't have the faintest idea if the various liquids used for slurries in various cultures during the last few thousand years actually employed that concept of chemical-mechanical polishing or CMP. I would be very surprised, however, if some of the old slurries didn't work that way. Of course, the master polisher had no idea why some slurries worked better than others, he just evolved better and better concotions.|
|It is clear by now, I hope, that
polishing your sword blade to a bright sheen is still not all that easy - if
you disdain brush polishing. On the other hand, polishing silicon wafers to
utter perfection, coming rather close to the figure above, is a standard process performed several 100.000
times a day. The roughness is less than 1 nm (or three atomic layers), and the
flatness (= large scale roughness) is less than 1 µm - on a scale of 300
mm = 300.000.000 µm! You need to polish your pyramid to almost optical
mirror quality in comparison.
How is it done? By chemical-mechanical polishing. And no, the few companies that can do it, won't tell you details about the slurries they use, and so on.
Meanwhile (for the last 20 years or so), this kind of precision polishing has been carried over to polishing some layers deposited on polished silicon wafers, including metals. "CMP", as it is called by all insiders, is actually a key process in semiconductor technology.
|Coming back to the beginning: I'm sure that the silicon polishing data are a lot better than what the best Japanese polishing masters could do. That doesn't belittle their achievements, it simply highlights that there is progress in some areas.|
|1)||Those Pharaohs were cool, man! Pharaoh Schepseskaf's pyramid (actually a mastaba) was named "Schepseskaf is cool" (see the article of Roman Guidacker in Sokar, 18, 2009, p. 26).|
Books and Other Major Sources
Defect Etching in Silicon
7.1.1 Finding Your Way in the Iron Carbon Phase Diagram
Early Metal Technology - 2. Silver and Lead
Critical Museum Guide: Dresden
Antique Texts Concerning Iron
Sword Polishing and Revealing the Pattern / Structure
The Frankish Empire And Its Swords
11.3.2 More to Pattern Welding
Science of Uniaxial Deformation
5.3.1 Grain Boundaries
Transmission Electron Microscopes
Hardware Around the Making of Metals and Their Proper Names
Theoderic's "Thank You" letter
Microscopes for Science
Scanning Electron Microscope
Moravian 9th Century Swords
© H. Föll (Iron, Steel and Swords script)